1 / 13

130 likes | 245 Vues

The Magnetic phase transition in the frustrated antiferromagnet ZnCr 2 O 4 using SPINS. Group B Ilir Zoto Tao Hong Yanmei Lan Nikolaos Daniilidis Sonoko Kanai Mitra Yoonesi Zhaohui Sun. Outline. Principle of triple axis neutron spectrometry

Télécharger la présentation
## The Magnetic phase transition in the frustrated antiferromagnet ZnCr 2 O 4 using SPINS

**An Image/Link below is provided (as is) to download presentation**
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.
Content is provided to you AS IS for your information and personal use only.
Download presentation by click this link.
While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
During download, if you can't get a presentation, the file might be deleted by the publisher.

E N D

**The Magnetic phase transition in the frustrated**antiferromagnet ZnCr2O4 using SPINS Group B Ilir Zoto Tao Hong Yanmei Lan Nikolaos Daniilidis Sonoko Kanai Mitra Yoonesi Zhaohui Sun**Outline**• Principle of triple axis neutron spectrometry • Sample properties: crystal and magnetic structure • Sample behavior: macroscopic (magnetic) properties • Neutron results: structural and dynamic information**A single point at a time**Sample Single Detector Neutron Source Analyzer Monochromator Conventional Triple-Axis Spectroscopy (TAS)**Sample**Position-Sensitive Detector D2qi hw ~1meV Flat Analyzer qai qa Q Probes scattering events at different energy and momentum transfers simultaneously Multiplexing Detection System for TAS qai = qa + D2qi = qa - atan(x sinqa/(L+xcosqa)) kfi = ta/2sinqai Qi = ki - kfi Survey (hw-Q) space by changing the incident energy and scattering angle**O**A B H = -JS Si. Sj nn Sample structure (ZnCr2O4) Space group Fd3m Lattice of B sites : Corner-sharing tetrahedra Edge-sharing octahedra ? Multiple energetically equivalent configurations: Geometric frustration**Magnetic Phase Transition in ZnCr2O4**QCW = 390 K TN = 12.5 K Phase transition**What information do we expect to get from neutron**scattering? • Static information: crystal structure and magnetic ordering, thus perform elastic scattering. • Dynamic information: what “excitations” do we observe and how they evolve with temperature, thus look for inelastic peaks • Dynamic and static correlations, thus look at peak linewidths. • How are the fluctuating spins in the spin liquid phase correlated with each other? • How do the spin correlations change with the phase transition?**I. Structural data**• Perform Q scan at zero energy transfer at several temperatures • Estimate Q resolution: ΔQFWHM0.2Å-1 • Estimate energy resolution: Δ(ћω) FWHM 0.2meV • Appearance of several magnetic peaks below the AF TN**(3/2,1,1/2)**(1,1,1) (3/2,1/2,1/2) (3/2,3/2,0) Structural insight gained • Position of (1,1,1) nuclear peak doesn’t shift • Several half integer indexed peaks appear • Comparable peak linewidths: Long range structural order**II. Dynamical data**• Scan for energy spectral weight at Q=1.5Å-1 • Shift in spectral weight from low (quasielastic)to high (inelastic) energy at TN. • T>TN: Thermal energy broadening. • T<TN: 4.5meV peak FWHM0.5meV (lifetime8ps). • What excitation is it? • Why the jump in energy?**II. More dynamical data**• Q scans at low and high T • Correlation length at ħ =1.5meV and T=15K is ~2.5 Å • Correlation length at ħ =4.5meV and T=1.5K is ~3.2 Å • Approximately same range of dynamic spin correlations; comparable to nearest neighbor distance ħ=1.5meV, T=15K ħ=4.5meV, T=1.5K**Resolution: The nature of the AF state.**• Antiferromagnetic spin hexagons form under TCW. • These can move independently (new degrees of freedom) • Still only spin liquid state can be formed (frustration) • Dynamical correlations of the formed hexagon span its size only • Frustration disappears due to crystal distortion at TN (lifting of degeneracy). • New AF ordered state appears. • Why the jump in energy? What is the Q dependence? To be continued…**Acknowledgements**Seung-Hun Lee Peter Gehring Sungil Park

More Related